Applied Geochemistry 116 (2020) 104580
Available online 2 April 2020
0883-2927/© 2020 The Authors. Published by Elsevier Ltd. This is an open access article under the CC BY-NC-ND license (http://creativecommons.org/licenses/by-nc-nd/4.0/).
Retention of technetium-99 by grout and backfill cements: Implications for
the safe disposal of radioactive waste
, Steve Langeb
, Guido Deissmannb
, Dirk Bosbachb
, Antoni E. Milodowskia,c
aDepartment of Chemistry, University of Surrey, Guildford, GU2 7XH, United Kingdom
bInstitute of Energy and Climate Research (IEK-6): Nuclear Waste Management and Reactor Safety, Forschungszentrum Jülich GmbH, 52425, Jülich, Germany cBritish Geological Survey, Keyworth, Nottingham, NG12 5GG, United Kingdom
dNational Physical Laboratory, Hampton Road, Teddington, Middlesex, TW11 0LW, United Kingdom
A R T I C L E I N F O Keywords: Technetium Adsorption Diffusion Cement A B S T R A C T
Technetium-99 (99Tc) is an important radionuclide when considering the disposal of nuclear wastes owing to its long half-life and environmental mobility in the pertechnetate (Tc(VII)) redox state. Its behaviour in a range of potential cement encapsulants and backfill materials has been studied by analysing uptake onto pure cement phases and hardened cement pastes. Preferential, but limited, uptake of pertechnetate was observed on iron-free, calcium silicate hydrates (C–S–H) and aluminate ferrite monosulphate (AFm) phases with no significant adsorption onto ettringite or calcium aluminates. Diffusion of 99Tc through cured monolithic samples, repre-sentative of cements being considered for use in geological disposal facilities across Europe, revealed markedly diverse migration behaviour, primarily due to chemical interactions with the cement matrix rather than dif-ferential permeability or other physical factors. A backfill cement, developed specifically for the purpose of radionuclide retention, gave the poorest performance of all formulations studied in terms of both transport rates and overall technetium retention. Two of the matrices, pulverised fuel ash: ordinary Portland cement (PFA:OPC) and a low-pH blend incorporating fly ash, effectively retarded 99Tc migration via precipitation in narrow, reactive zones. These findings have important implications when choosing cementitious grouts and/or backfill for Tc-containing radioactive wastes.
Technetium-99 (99Tc) is a low energy (Emax ¼ 0.29 MeV), beta-
emitting product of uranium fission in a nuclear reactor. It is also pro-duced, in smaller quantities, from isomeric transition of the diagnostic nuclear medicine isotope 99mTc. Given its long half-life (211,100 years; Brown et al., 2018), high yield (6.1% for thermal neutron fission of 235U; Brown et al., 2018) and environmental mobility (Wildung et al., 1978;
Schulte and Scoppa, 1987; Lloyd et al., 2000; Masters-Waage et al., 2017), retention of 99Tc is an important factor to consider when
assessing the safety performance of radioactive waste repositories. In addition to its occurrence as a fission product in spent nuclear fuels (Kleykamp, 1988; Bruno and Ewing, 2006; Carbol et al., 2012; Lewis et al., 2012), it typically occurs in operational wastes such as ion-exchange resins, contaminated liquids, filters and sludge (Westsik et al., 2014; Ochs et al., 2016) and therefore, some form of treatment is
required to render it into a passive, solid waste form. Cement is the most commonly used encapsulant for reasons of cost or ready availability and also because the behaviour of technetium during high-temperature thermal treatment such as vitrification is problematic; it volatiles and only a fraction is retained in the glass (e.g. Childs et al., 2015; Pegg, 2015; Luksic et al., 2015; Kim and Kruger, 2018). Unfortunately how-ever, data on the interactions of technetium with cementitious phases and hardened cement pastes (HCP) is limited.
Retardation of radionuclides in cement can occur by three principal mechanisms; precipitation of insoluble phases, incorporation into existing or newly-formed mineral phases and surface adsorption ( Jant-zen et al., 2010; Westsik et al., 2014; Ochs et al., 2016). Thus, the ca-pacity of a cement grout or backfill to retain any given radionuclide will vary depending on the chemical speciation of the nuclide and the properties of the cement. The potential for precipitation of cationic species in high pH cementitious pore waters is well known: similarly,
* Corresponding author. Department of Chemistry, University of Surrey, Guildford, GU2 7XH, United Kingdom.
E-mail address: email@example.com (D. Read).
Contents lists available at ScienceDirect
journal homepage: http://www.elsevier.com/locate/apgeochem
uptake in cementitious systems by adsorption to calcium silicate hydrate (C–S–H) phases, uptake into the C–S–H interlayer, exchange of Ca ions in the C–S–H structure or incorporation into layered double hydroxide (LDH)-type phases, such as AFm, (e.g. Atkins et al., 1992; Evans, 2008;
Ochs et al., 2016). However, it is often assumed, at least in safety as-sessments, that anionic species will be much more mobile (e.g. Posiva, 2012; SKB, 2015). Recent research has challenged this assumption by demonstrating the precipitation and/or mineralisation of selenium (Felipe-Sotelo et al., 2016a), chlorine (Milodowski et al., 2013; van Es et al., 2015) and iodine (Felipe-Sotelo et al., 2014). Moreover, redox-sensitive, anionic radionuclides of, for example, selenium or technetium, may be precipitated in less soluble, reduced forms, depending on conditions, e.g. in slag-rich formulations. Nevertheless, retention of anionic species has not been studied to the same extent as cations and there is no guarantee that findings for ordinary Portland cement (OPC) will be valid for the wide variety of blended cement for-mulations under consideration in nuclear waste management. Changes associated with degradation of the cement matrix over time and the presence of additives such as superplasticisers further complicate the issue (Ochs et al., 2016; Isaacs et al., 2018).
Technetium is a redox sensitive element and can occur in nuclear waste streams in either the Tc(IV) or Tc(VII) state, depending on the redox potential of the solution and pH (Fig. 1). Speciation calculations suggest that its solubility will be in the range 10 7 - 10 6 mol dm 3, controlled by hydrous TcO2, in the presence of corroding iron from steel
drums (Eh ~ - 800 mV) and over the pH range anticipated for cemen-titious conditions. Irrespective of the redox state, dissolved Tc in cementitious environments will be present predominantly in an anionic form either as TcO(OH)3- or as TcO4; the pertechnetate ion (TcO4) is
favoured under more oxidising and also hyper-alkaline conditions (Eriksen et al., 1993; Cui and Eriksen, 1996; Burke et al., 2005; Warwick et al., 2007; Hallam et al., 2011).
Previous studies indicate that pertechnetate is poorly retained in both young and mature Portland cements due to the negatively charged surfaces of C–S–H (Tallent et al., 1987; Brodda and Xu, 1989; Smith and Walton, 1993; Mattigod et al., 2001, 2004; Evans, 2008; Corkhill et al., 2012). The major mechanism of retention of technetium in blended cements was found to be reduction to less mobile Tc(IV) or Tc(0) by reducing agents present in those materials. Tallent et al. (1987) studied the influence of grout composition on the leachability of technetium-containing cementitious matrices. They demonstrated that leachability decreases with increasing mix ratio, grout fluid density and blast furnace slag (BFS) content. Later, Gilliam et al. (1990) showed that
the effective technetium diffusivity of cement-based waste forms de-creases by five orders of magnitude on the addition of BFS. A further decrease of the leach coefficient in water and brine was achieved by addition of sodium sulphide, as reported by Brodda and Xu (1989), who concluded that technetium appeared to be chemically bound. Thermo-dynamic calculations carried out by Smith and Walton (1993) suggested that technetium leachability decreases owing to reaction with the sulphur present in BFS and formation of Tc2S7. The addition of a limited
amount of BFS led to a significant improvement in leach test perfor-mance but further BFS loading had only a marginal effect.
Allen et al. (1997a,b) conducted extended X-ray absorption fine structure (EXAFS) studies on the effect of blast furnace slag and metal sulphides on technetium speciation. Their results demonstrated that the addition of BFS to a cement formulation leads to only partial reduction of any pertechnetate anions present, whereas the addition of Na2S or FeS
results in complete reduction to the less mobile Tc(IV). They concluded that sulphide-containing species rather than elemental sulphur are the active reducing agents in BFS. These authors also measured interatomic Tc–S and Tc–Tc distances in the presence of Na2S or FeS, observing bond
distances in agreement with an oligomeric structure similar to that found in TcS2 (Allen et al., 1997a, b).
Not all authors agree that reduction to Tc(IV) is necessary for tech-netium immobilisation. Berner (1999) suggested that binding and/or incorporation of TcO4 into the alumina ferric mono/tri-sulphate
(AFm/AFt) phases of cement systems could also be expected, by anal-ogy to other oxo-anions such as SO42 or MoO42 , and possibly also
SeO32 . This has been tentatively confirmed in the case of ettringite by
EXAFS and X-ray absorption near edge structure (XANES) analysis of a hydrated lime and sulphate-rich simulant waste form (Saslow et al., 2018). The resulting spectra show that TcO4 substitutes directly for
sulphate in the crystal lattice. The findings imply reduction to Tc(IV) is not essential for technetium immobilisation, which is important as ox-ygen diffusion and re-oxidation of Tc(IV) in a waste form might occur over longer timescales. Indeed, Smith and Walton (1993) concluded that the diffusion of oxygen into HCP or concrete would oxidise Tc2S7 to the
highly mobile TcO4, which could then diffuse out from the waste.
Layered double hydroxides have also been suggested as potential host phases for technetium in its anionic form. Several natural minerals are known to incorporate technetium, for example fougerite (green rust), a layered double hydroxide-carbonate belonging to the hydro-talcite group, with the formula ([Fe2þ4Fe3þ2(OH)12][CO3]⋅3H2O), as
well as potassium metal sulphides. A good overview of these potential host phases is given by Luksic et al. (2015).
Finally, some radioactive waste disposal concepts are considering cements not only as grouts but as potentially suitable backfill materials and as a component in specific high-level waste containers (e.g. Bel et al., 2006; NAGRA, 2002, 2008; Verhoef et al., 2014). Clearly, the situation where the cementitious barrier is already in place before encountering migrating radionuclide species is very different from the intimate mixing of unhydrated cement pastes with aqueous wastes. The aim of the present work is to assess both situations by considering the uptake of 99Tc in a) a number of individual cement phases and HCP and
b) diffusion of 99Tc through cured monolithic samples representative of those being considered for use in geological disposal facilities across Europe.
The solids of interest fall into two categories, single cement mineral phases and hardened cement pastes (HCP); both were used for batch adsorption tests with the latter also employed for through-diffusion studies. Cement minerals comprised C–S–H with calcium: silica ratios of 0.9 and 1.4 (denoted C–S–H0.9 and C–S–H1.4, respectively), ettrin-gite (AFt, Ca6Al2(SO4)3(OH)12⋅26H2O), hydrogarnet (C3AH6, Ca3
A-l2(OH)12), portlandite (Ca(OH)2), calcite (CaCO3) and two AFm phases
(Ca4Al2(OH)12 (X2 )⋅6H2O) namely, AFm-SO4 and AFm-CO3. The Fig. 1. Eh-pH diagram for Tc species in aqueous systems (Tc ¼ 10 6 M(left), Tc
¼10 9 M(right). Aqueous species are shown in light blue, solids in light grey. Thermodynamic database: ThermoChimie Version 9b0; Giffaut et al., 2014;
Griv�e et al., 2015). (For interpretation of the references to colour in this figure legend, the reader is referred to the Web version of this article.)
synthesis of these model phases, representative of hydration products in HCP, were carried out following established procedures (i.e. C–S–H:
Atkins et al., 1992; AFm: Baur et al., 2004 and Matschei et al., 2006; ettringite: Atkins et al., 1991 and Baur et al., 2004). The methods are described in detail in Lange et al. (2018). In order to avoid carbonation of the material, synthesis of the phases, sample preparation and storage were carried out in an argon glove box (<10 ppm CO2). After
purifica-tion, structure and purity of the model phases as well as the phase as-semblages present in HCP samples were characterised by powder X-ray diffraction spectroscopy (XRD), using either a D8 Advance (Bruker AXS GmbH) with a θ-θ geometry or a D4 Endeavor (Bruker AXS GmbH) with a θ-2θ geometry, employing CuKα-radiation. Microstructure and phase
morphology were investigated by Scanning Electron Microscopy (SEM; FEI Quanta 200F) equipped with a field emission cathode. Energy dispersive X-ray spectroscopy (EDX) was performed using an Apollo X Silicon Drift Detector (SDD) from EDAX. SEM/EDX analyses were car-ried out in low vacuum mode (60 Pa) to avoid coating the samples with carbon or gold. The characteristics of the phases are described in detail elsewhere (Lange et al., 2018).
Sorption distribution ratios (Rd values) and technetium uptake
ki-netics on the model phases were determined in static batch experiments under anoxic conditions, employing different test solutions. Generally, 20 cm3 LDPE bottles were used at solid to liquid (S/L) ratios of
0.005–0.04 kg dm 3, depending on the aim of experiment. In the first set of experiments, weighed amounts of dried solids were equilibrated with deionised water (18.2 MΩ) to obtain equilibrium solutions (ES); the suspensions were stored at room temperature for up to 14 days under anoxic conditions to achieve equilibrium between aqueous and solid phases. Subsequently, solid and liquid phases were separated by filtra-tion. The pH of the respective equilibrium solutions is provided in
Table S1 in the Supplementary Information. pH measurements were performed with a Metrohm Unitrode electrode with integrated Pt- temperature sensor, suitable for measurements between pH 0 and 14. In addition to solutions equilibrated with the respective solids, experi-ments using an alkali-rich artificial young cement water (ACW, pH > 13) and a solution saturated with portlandite (CH, pH ~12.5) were per-formed to address conditions representative of concrete degradation stages I and II (Glasser, 2011; Hoch et al., 2012; Ochs et al., 2016). Artificial young cement water was prepared by filtration and dilution of highly concentrated sodium and potassium hydroxide solutions, subse-quently saturated with Ca(OH)2 (Wieland et al., 1998). The resulting
solution containing 0.114 mol dm 3 Na and 0.18 mol dm 3 K had a pH
of 13.3; the saturated portlandite solution (CH) contained 0.19 mol dm 3 Ca at pH 12.3.
For the sorption experiments, defined amounts of the respective fresh model phases were added to the equilibrium solutions at a S/L-ratio of 0.04 kg dm 3 and stored for an additional 14 days, before 99Tc was added as a tracer in the form of pertechnetate at concentrations ranging from 10 5 M to 10 7 M. Solution activity concentrations were
moni-tored for up to 100 days by liquid scintillation counting (LSC) to ensure steady state had been reached; the bottles were shaken by hand regu-larly. To avoid removing solution during sampling, a separate test batch was used for each time step in those experiments addressing uptake kinetics. The pH in the respective solutions was found to be constant over the duration of the experiments. The timeframes for experiments to determine final Rd values were defined based on the uptake kinetics.
Adsorption of pertechnetate to reaction vessels and filters was tested prior to the experiments and found to be negligible.
LSC measurements were performed using a 1220 Ultra low level Quantulus™ LSC device (Perkin Elmer). Sample aliquots of 50 μL were
diluted in a 20 cm3 polyethylene vial with 15 cm3 Hionic-Fluor or
Ul-tima Gold™ LSC-cocktail (Perkin Elmer). Liquid and solid phases were separated using USY-1 ultrafilters (10,000 Da, Advantec) prior to anal-ysis of the concentration in solution. At the end of the batch sorption experiments the solids were separated by filtration and analysed by XRD and SEM-EDX.
The uptake of technetium by the solid phases is described here in terms of a distribution ratio Rd between 99Tc adsorbed by the solids
(99Tcsorbed) and the 99Tc remaining in solution (99Tc solution) as:
Rd¼ 99Tc sorbed 99Tc solution (eq. 1) and calculated according to:
Rd¼ 99Tc initial 99Tct 99Tc t V m (eq. 2)
where 99Tcinitial is the initial concentration of 99Tc in solution (Bq or M),
and 99Tct the concentration at time t, respectively; V is the volume of the
liquid phase and m the mass of solid used in the experiment. Estimation of uncertainties for the distribution ratio (Rd) was performed using the
statistical software of the LSC device, comprising uncertainties resulting from both the sample measurement and the background spectra. Errors arising from each step of the experimental procedure (e.g. weighing and pipetting) were included using Gaussian error propagation.
Similar batch experiments were carried out on two HCP samples, CEM I and a low-pH reference cement blend used for benchmarking purposes in the pan-European CEBAMA project (Grambow et al., 2020), produced according to a specification provided by Valtion Teknillinen Tutkimuskeskus (VTT), Finland (Vehmas et al., 2017, Vehmas et al., 2020). CEM I HCP specimens were prepared in a glove box under argon atmosphere (<10 ppm CO2), using a commercially available Portland
cement (CEM I 32.5 R; Heidelberger Zement) at a water/cement ratio (w/c) of 0.4 dm3 kg 1. The cement pastes were cast in cylindrical
moulds and cured for at least 28 days submerged in water under anoxic conditions; the demoulded monoliths were subsequently stored under argon atmosphere. In addition to OPC, the Cebama reference blend low pH cement formulation comprised blast furnace slag and silica fume as well as quartz filler (Vehmas et al., 2017; cf. Table 2). This HCP, pro-vided by VTT, had been prepared with a w/c-ratio of 0.25 dm3 kg 1 and
hydrated for 90 days in a saturated KOH solution to prevent leaching. The HCP was mechanically crushed, followed by multipoint N2-BET
surface area determination, using a Quantachrome Autosorb 1. Adsorption experiments with HCP were performed in an analogous manner to the experiments with model phases at a S/L-ratio of 0.02 kg dm 3, using crushed materials in solutions pre-equilibrated for 14 days
with the respective HCP. The pH of the equilibrated solutions used in the experiments was 12.6 (CEM I) and 12.5 (Cebama low-pH reference blend), respectively. The rather low equilibrium pH in the system with crushed CEM I HCP in comparison to the pH expected in young Portland cement-based systems is attributed to the low S/L-ratio used in the ex-periments and thus, the low alkali inventory.
Five cement blends were included in the through-diffusion study; an ordinary Portland cement (OPC; CEM I), a ground granulated blast furnace slag: ordinary Portland cement blend (GGBS:OPC), a pulverised fuel ash blend (PFA:OPC), a bespoke backfill material (NRVB, Nirex Reference Vault Backfill) and the reference cement blend used for benchmarking purposes noted above, provided by VTT, Finland ( Veh-mas et al., 2017, 2020).
The CEM I 42.5N, obtained from Hanson Cement, Ribblesdale, UK with a fineness of 347 m2 kg 1 and specific gravity of 3.13 g cm-3,
complies with both BS EN 197–1:2011 and a technical specification (Angus et al., 2011) for the supply of powders for the encapsulation of intermediate level radioactive waste (ILW) in the UK. The GGBS, with fineness of 517 m2 kg 1 and specific gravity of 2.91 g cm-3, was obtained from Hanson Cement, Scunthorpe, UK (Isaacs et al., 2018); it complies with BS EN 15167–1:2006. Hydrated lime (Lafarge) complies with the requirement of BS EN 459-1 to be building lime standard. Limestone flour is available commercially (NAF Limestone Flour, NAF, Monmouth, UK). The constituents of the Cebama reference blend were provided by VTT, as noted above. The Finnish CEM I (Cementa) has a fineness of 310
m2 kg 1 and complies with the EN 197-1 standard. Finnish GGBS
(Finnsementti) has a fineness of �275 m2 kg 1 and meets the technical
specification of EN 15167–1:2006. Silica fume was also derived from Finnsementti and meets the standard of EN 13263–1:2009. The water/cement ratio was increased slightly from that specified by VTT to provide a workable cement in the absence of plasticiser (Isaacs et al., 2018).
X-ray fluorescence (XRF) analysis was used to determine the major components of these starting materials (Table 1). The formulations used for each of the HCP samples are detailed in Table 2.
The powders were mixed using a bench-top conical mixer in a polypropylene hexagonal barrel (Pascall Lab-mixer II, Pascall Engi-neering) until homogeneous. A series of pre-equilibrated waters for use in the experiments was prepared by adding 50 g of each HCP powder above to 1 dm3 deionised water under N
2 atmosphere. The suspension
was agitated daily to prevent sedimentation. After 28 days the solids were removed by filtration and the solutions analysed by ion chroma-tography (Table 3).
An aliquot of pre-equilibrated solution was added to each HCP powder at a liquid/solid ratio of 0.45 and mixed for 5 min by hand. The mix was then poured into 50 cm3 polypropylene containers, gently
tapped to remove any trapped air bubbles and left to set for 24 h before removing the cylinders from the moulds. The samples were cured in sealed containers for a period of 28 days before use in the diffusion experiments. After the curing period, the blocks were removed from the solution and a well drilled centrally along the longitudinal axis of the cylinders; the depth of the central well was 30 mm with a diameter of 10 mm. The top and bottom surfaces of the block were sealed with wax. The cement cylinders had a diameter of 40 mm and a length of 40–45 mm. The diffusion of 99Tc through cured HCP samples was assessed using
an experimental protocol described previously (Felipe-Sotelo et al., 2014, 2016a,b; van Es et al., 2015). An aliquot of 99Tc (1.6 kBq) as
ammonium pertechnetate in 1 cm3 pre-equilibrated cement water was
spiked into the central well of the block, which was then sealed and submerged in 200 cm3 of the same pre-equilibrated water used for
curing (Fig. 2). The cement blocks, sealed in individual Nalgene con-tainers, were kept in a N2-atmosphere glove box throughout the
exper-iment and during sampling. All experexper-iments were carried out in duplicate.
Movement of 99Tc through the block was monitored by measuring
the equilibrated water surrounding the block by taking 1 cm3 aliquots
initially on a daily basis and then weekly. The solutions were filtered before use through qualitative filter paper (Fisher Scientific). The ac-tivity in the samples was determined by LSC (Packard 2100 TR, Liquid Scintillation Analyzer) in the energy range between 20 and 200 keV after the addition of liquid scintillation cocktail (Goldstar, Meridian, UK) at a sample to scintillant ratio of 1:10. Each sample was agitated on a whirlimixer for 30 s and the samples were stored in a dark room for a minimum of 24 h before measurement.
At the end of the equilibration period, the cylinders were removed from solution and cut longitudinally with a diamond masonry saw in order to determine the migration profiles of the 99Tc by digital laser-
photostimulated luminescence (LPSL) autoradiography, using storage
phosphor imaging plates (IP). The IP comprise a layer of microcrystal-line Eu-doped barium fluorobromide (BaFBr:Eu2þ) photo-stimulable
phosphor layer bonded to a polyester plastic support. Incident radia-tion excites Eu2þfrom its ground state to the metastable Eu3þ, liberating
electrons to the conduction band, which are trapped in crystal defects (hole-electron pairs or F-centres) in proportion to the incident radiation (Zeissler, 1997; Gonzalez et al., 2002; Takahashi, 2002; Leblans et al., 2011). Stimulation of the phosphor by red laser light excites the stored electrons to the conduction band, where they recombine with Eu3þions,
releasing energy in the form of blue light as a result of 5d-4f transition when the excited electron falls to the ground state in the Eu2þion. This emitted light is detected by a photomultiplier and is proportional to the radioactivity that the phosphor was exposed to (Takahashi, 2002; Leb-lans et al., 2011). The IP technique cumulatively detects alpha-, beta- and gamma-radiation, as well as background cosmic radiation.
The IP were initially exposed to bright white fluorescent light for 20 min to erase any previously-acquired residual latent image and back-ground (gamma and cosmic) radiation signal. LPSL autoradiography images were produced by placing the flat surfaces of the cut cylinders directly onto Fuji BAS-MP2025P general purpose polyurethane-coated IP for 4 h in a light-tight box. Following exposure, the IP were care-fully removed under darkroom conditions and scanned using an Amer-sham Biosciences (GE Healthcare Ltd) STORM™ 860 digital fluorescence laser scanner, with red laser light (635 nm) and a 650 nm low-pass wavelength filter, to release the stored energy and record the latent image. The IP were scanned at a 50 μm pixel resolution and the
resultant digital autoradiography images were recorded as 16-bit ‘GEL- format’ image files. These employ a square root algorithm coupled with a ‘scaling factor’ to accommodate the wide dynamic range of the IP, and compresses the 100,000 possible levels of signal resolution into the more limited range available in a standard TIFF (tagged image file) image. This provides higher signal resolution at the low end where changes in signal are more critical. However, the resulting raw data stored within each pixel of a GEL image file are non-linear. The ‘GEL-format’ LPSL autoradiography images were initially processed using the ImageQuant TL (v.2005) software package (Amersham Biosciences, 2005). The GEL files were subsequently processed to produce detailed, 16-level colour-contoured autoradiographs using the FiJi (ImageJ) (v. 1.48k 15 December 2013) public-domain open-source software package ( Ras-band, 2013). This was coupled with the ‘Linearise GelData’ software ‘plug-in’ (Cathelin, 2012) to square and scale the GEL file data (default scale factor for ‘GEL-format’ files is 1/21025) in order for the images to be displayed correctly as quantitative linear colour-contoured intensity images. ImageQuant TL (v.2005) was also used to plot the variation in radioactivity (determined as image ‘diffuse density’) across the cement blocks from the LPSL autoradiography images, along ‘lane profiles’ drawn perpendicular to the walls of the well.
For comparison purposes, similar experiments were carried out for each HCP formulation using a nominally conservative tracer, tritiated water (HTO). A total activity of approximately 5000 Bq (Perkin Elmer) was added to the central well of the cement blocks. As for the technetium experiments, HTO diffusion was assessed in duplicate and breakthrough was determined by LSC.
Major elements in the constituents used to prepare the cement pastes for through-diffusion experiments.
Cement Powder CaO [wt%] SiO2 [wt%] Al2O3 [wt%] SO3 [wt%] MgO [wt%] Fe2O3 [wt%] K2O [wt%] P2O5 [wt%] TiO2 [wt%] MnO [wt%]
CEM I 66.27 17.86 4.78 3.98 2.75 2.65 1.52 nd 0.2 nd PFA 3.86 48.66 25.97 1.82 1.27 12.36 5.05 0.18 0.84 nd GGBS 42.93 31.92 11.40 4.10 6.76 0.45 1.01 nd 0.41 0.59 Hydrated Lime 97.75 1.37 0.35 nd 0.20 nd 0.33 nd nd nd Lime Flour 96.57 1.70 0.71 0.18 0.29 0.16 0.39 nd nd nd Silica Fume 1.46 93.10 1.44 0.47 0.88 0.91 1.73 nd nd nd CEM I (VTT) 67.72 17.60 3.42 3.81 0.6 5.17 1.3 nd 0.17 0.21 GGBS (VTT) 43.13 32.3 9.85 3.68 7.40 0.74 1.20 nd 1.36 0.34 nd – not detected.
3. Results and discussion
3.1. Uptake of 99Tc by individual cement phases
The kinetics of Tc(VII) uptake by the model hydration phases in the various solutions (i.e. with or without alkalis) were determined at a S/L- ratio of 0.005 kg dm 3 for up to 100 days; the results of these adsorption
tests as a function of time are shown in Fig. S1 in the Supplementary Information. Within experimental error, the measured TcO4
concen-trations in solution were similar to the initial tracer concentration (10 7
M), indicating only minor retention by the pure model phases. Thus, calculated Rd values encompass negative values and could not be
distinguished from background. Where uptake was observed, the kinetic tests indicate a fast uptake process, leading to equilibrium within a few days.
Equilibrium Rd values determined after 28 days at a S/L ratio of 0.04
kg dm 3 are given in Table 4 and shown graphically in Fig. S2 in the Supplementary Information. Apparent differences in the distribution ratios (Rd ¼4.5 dm3 kg 1 for C–S–H0.9 and Rd ¼2.3 dm3 kg 1 for the more Ca-rich C–S–H1.4) are small and may not be significant. The sorption of oxyanions such as IO3or MoO4to C–S–H is often attributed
to electrostatic adsorption to the C–S–H surface (e.g. Bonhoure et al., 2002; Ochs et al., 2016). Thus, uptake of these anions should increase with increasing Ca/Si ratio in C–S–H, since the zeta potential of C–S–H is zero for Ca/Si ¼ 1.2 and negative at Ca/Si < 1.2. Atkins et al. (1992) also predicted that the increasingly positive surface charge at Ca/Si > 1.2 should result in more pronounced uptake of anions. However in our experiments, the higher affinity of TcO4 towards C–S–H with lower
Ca/Si-ratio, consistently corroborated by the adsorption isotherms ob-tained at dissolved TcO4 concentrations between 10 5 and 10 8 M
(Fig. 3), does not reflect the trend observed for other anions. Considering
Formulations of HCP samples used in the through-diffusion experiments.
Cement Blend OPC PFA GGBS Hydrated Lime Lime Flour Silica Fume Quartz Water/cement ratio
CEM I 1 0.45 PFA:OPC 1 3 0.45 GGBS:OPC 1 9 0.45 NRVB 1 0.38 1.1 0.55 Cebama 1 0.62 1.05 1.1 0.45 Table 3
Composition of aqueous solutions equilibrated with the HCP used in the through-diffusion experiments.
Cement Blend Cl mg kg1 SO 4 mg kg 1 NO3 mg kg 1 Na mg kg1 K mg kg 1 Mg mg kg 1 Ca mg kg1 pH Eh [mV] CEM I 18.0 36.9 18.1 267.6 453.3 nd 1388.4 12.8 14 PFA:OPC 14.4 31.0 16.3 129.8 195.2 39.0 675.8 12.3 503 GGBS:OPC 16.9 34.7 17.6 68.6 70.2 nd 299.6 12.8 414 NRVB 16.0 33.6 17.2 172.5 224.7 66.3 1374.3 12.9 129 Cebama 24.0 50.3 20.4 189.7 202.3 137.0 1046.6 12.7 454 nd – not detected.
Fig. 2. Schematic of the radial diffusion experiments using various HCP.
Distribution coefficients (Rd) for the uptake of99Tc by cement hydration phases in various solutions (ES: equilibrium solution; ACW: artificial young cement water (pH 13.3); CH: saturated portlandite solution (pH 12.3)).
Phase Rd [dm3 kg 1] ES ACW CH C–S–H 0.9 4.5 � 2.7 4.1 � 2.7 na C–S–H 1.4 2.3 � 2.4 1.9 � 2.3 na AFm-SO4 4.0 � 1.9 0.7 � 1.5 0.6 � 1.5 AFm-CO3 2.3 � 1.7 na 1.1 � 1.5 Ettringite 0.6 � 0.9 0.6 � 0.9 0.6 � 0.9 Hydrogarnet C3AH6 0.6 � 1.6 0.6 � 1.6 1.0 � 1.7 Portlandite na na 1.0 � 2.2 Calcite 0.6 � 2.2 na 0.8 � 2.2 na – not analysed.
Fig. 3. Sorption isotherms for pertechnetate uptake by C–S–H0.9 and C–S–H1.4.
the generally low distribution ratios obtained, the higher affinity of pertechnetate to C–S–H0.9 might be attributable here to differences in the surface area of the synthetic C–S–H (C–S–H0.9 ¼ 125 m2 g 1;
C–S–H1.4 ¼ 109 m2 g 1; Lange, 2019). The experiments performed in
young cementitious water (ACW) indicated (virtually) no effect of pH and alkali concentration in solution on pertechnetate uptake by the synthesised C–S–H phases.
In addition to C–S–H, some, albeit limited, uptake of pertechnetate was apparent for AFm-SO4 (Rd ¼4.0 dm3 kg 1) and AFm-CO3 (Rd ¼2.3 dm3 kg 1). The uptake of the pertechnetate anion by AFm-phases could
be due to surface adsorption, edge sorption to the octahedral layers or to exchange for the interlayer anion, similar to the uptake of MoO4 or
SeO4, as described by Ma et al. (2017, 2019). The potential for anion
exchange in the interlayer was probed by XRD measurements, since the size of the pertechnetate oxo-anions (ionic radius of Tc(VII): 37 p.m. for coordination number 4 (Shannon, 1976); Tc–O bond length 173 p.m. (Lukens et al., 2003; Weaver et al., 2017)) is larger than that of sulphate ions (ionic radius of S(VI): 12 p.m. for coordination number 4 (Shannon, 1976); S–O bond length: 147 p.m. (Hawthorne et al., 2000)). However, no changes in the interlayer spacing of the AFm phases or new re-flections attributable to the exchange of pertechnetate for the interlayer anions were observed. These findings probably reflect the low degree of uptake of pertechnetate by the AFm phases, bearing in mind that a change in the extent of hydration (i.e. the number of water molecules in the interlayer) accompanying the anion exchange process would also affect the interlayer distance. Generally, for the exchange of interlayer anions in layered double hydroxides and AFm-type phases, divalent anions (e.g. CO32 or SO42 ) are preferred over monovalent anions (e.g.
TcO4, Cl , IO3, I ; Jantzen et al., 2010). However, the slightly lower
pertechnetate uptake by AFm-CO3 compared to AFm-SO4 might indicate
that exchange of the (tetrahedral) TcO4for the planar CO32--anion is less
favoured compared to exchange with the tetrahedral SO42--anion. The
less pronounced pertechnetate uptake by the AFm phases in young cement water and portlandite buffered solutions suggests a slight dependence on solution pH and composition.
The uptake of pertechnetate by all other model phases tested was found to be negligible (Table 4). The Rd value determined for systems
containing ettringite was <1 dm3 kg 1, indicating practically no uptake
of TcO4 due to exchange for the sulphate groups of this phase. This
suggests that the uptake mechanism proposed by Berner (1999) does not contribute to Tc(VII) retention in cementitious systems in the case of pre-existing ettringite. In contrast, a partial incorporation of pertech-netate in ettringite precipitating in the presence of dissolved TcO4 ions
is to be expected (e.g. Saslow et al., 2018), which would be relevant, for example, with respect to the immobilisation of liquid waste streams by cementation.
3.2. Uptake of 99Tc by HCP
Results of the batch sorption experiments using crushed HCP are shown in Fig. 4. Tc(VII) uptake by HCP reached a steady state after only 1 day with rather low Rd values < 10 dm3 kg 1. These findings are in
good agreement with the stated high mobility and low retention of TcO4
in cementitious environments in the absence of reductants (e.g. Ochs et al., 2016). As anticipated from the batch uptake experiments with single phases, the distribution ratios of HCP based on CEM I were somewhat lower than those of the low-pH paste based on the Cebama reference blend. This can be explained by the lower Ca/Si ratio of the C–S–H in the Cebama reference blend HCP, and the higher content of Fe (II) and/or sulphides in this material, due to the GGBS in the cement formulation. The latter could lead to Tc retention by reduction of mobile Tc(VII) to Tc(IV) and consequent formation of TcO2 or Tc-sulphides (e.g. Allen et al., 1997b; Warwick et al., 2007; Westsik et al., 2014; Master-s-Waage et al., 2017).
In experiments using crushed CEM I HCP, the solution pH remained constant throughout (pH ~12.6). Owing to the low S/L-ratio in the experiment and leaching of the alkalis, as indicated by a solution pH probably controlled by portlandite dissolution, the material corresponds to a slightly degraded cement in stage II (Lange et al., 2018). In contrast, with experiments using HCP prepared from the Cebama reference low pH cement blend, the solution pH dropped from an initial 12.5 to 11.8 after 75 days, indicating ongoing hydration of this material. This would lead to continuous formation of C–S–H with low Ca/Si-ratios from remaining unreacted clinker phases (silica fume and blast furnace slag (GGBS)), as predicted by the hydration model of Idiart (2017).
Retardation of radionuclides by hardened cements reflects a com-bination of physical and chemical processes. The experiments conducted with tritium represent an attempt to distinguish between the two. This is obviously an over-simplification as, although often regarded as a con-servative tracer, tritium will undergo isotopic exchange for hydrogen bound in solid phases, particularly C–S–H and thus, the slower its movement, the greater the scope for interaction; i.e. the physical and chemical aspects are intimately coupled. Nevertheless, the difference in tritium transport rates between respective cement formulations should be, as a first approximation, primarily a function of HCP permeability. The results demonstrate that initial tritium breakthrough is rapid, as expected, with some 3H detected in the solution surrounding the blocks at the first sampling point (Fig. 5). Activity concentrations for the PFA: OPC and NRVB blends then approach input levels after 14 days. Transport through the Cebama reference blend is slower, taking 28 days to reach a C/C0 value of 0.8 with CEM I and GGBS:OPC cements taking
progressively longer; indeed, concentrations are apparently still increasing at the end of the experiment (270 days). On this basis, if technetium migration were to be unaffected by chemical interactions between solution and the cement solids, the rate of transport would be expected to decrease in the order PFA:OPC � NRVB > Cebama ≫ CEM I �GGBS:OPC (Fig. 5).
The findings for tritium are borne out with NRVB and, to an extent with PFA:OPC, though the latter displays more complex behaviour (Fig. 6). In the case of NRVB, 99Tc appears in the surrounding solution after just one day, implying minimal retention. Levels reach a C/C0 value
above 0.7 after just one month and steady state is maintained at C/C0 ¼ 0.8 for the remainder of the experiment. Breakthrough also occurs rapidly with the PFA:OPC formulation; however, the peak in C/C0
oc-curs after one month, followed by a slow and progressive decline (Fig. 6). This was unexpected and suggests that the 99Tc released to
solution is subsequently re-adsorbed or precipitated by the cement. CEM I and GGBS:OPC gave similar profiles as for tritium, slowly increasing over 270 days, albeit at much lower C/C0 values, (reaching
only 0.2 and 0.3, respectively). Finally, measurements of 99Tc activity in the solution surrounding the Cebama reference blend show no sign of breakthrough after 270 days (Fig. 7). This represents the most pro-nounced difference with tritium patterns (cf. Fig. 5) and the clearest indication of chemical retention displayed by all of the cements inves-tigated in the study.
At the completion of the experiments, the blocks were cut
longitudinally to reveal the centre of the cylinders, allowing the migration profile of 99Tc to be examined from the central well to the
outer edge of each block using digital autoradiography. Autoradiog-raphy of the NRVB reveals that the level of radioactivity within the cement is indistinguishable from background (Fig. 8a). This is in accordance with the solution analyses and demonstrates that this ma-terial has very little capacity to retain technetium. Autoradiographic images for CEM I and GGBS:OPC display broadly similar low levels of dispersed activity throughout the blocks (Fig. 8b and c), again consistent with migration of 99Tc through the cement and a limited degree of
retention. In the case of CEM I, the low level of radioactivity appears to be uniformly distributed, with the exception of a few small localised ‘hot-spots’ (Fig. 8b) that possibly correlate with discrete (dark) cement clinker particles. In the GGBS:OPC block, the distribution of radioac-tivity is more elevated in a diffuse band close to the wall of the central well, reaching a peak at a depth of 2–3 mm into the cement matrix. Thereafter, the activity gradually decreases to background levels to-wards the edge of the block (Fig. 8c).
Much greater retention of 99Tc is apparent in both the Cebama
reference blend and PFA:OPC cements. Autoradiography of the former (Fig. 9a) revealed a region of high activity close to the central well, with a very pronounced peak in activity at a depth of 1.5–2 mm into the cement, decreasing to background level between 9 and 10 mm from the well wall (features labelled ‘y’ in Fig. 9a(ii)). There is no evidence from autoradiography of 99Tc transport further into the block, consistent with
the solution analyses noted previously, where no breakthrough was observed into the surrounding solution with the Cebama reference blend. The autoradiographic images for PFA:OPC are interesting and point to more complex behaviour. Low-level activity from 99Tc is present
throughout the block and shows a generally decreasing trend from the central well to the surface (Fig. 9b). Superimposed on this trend is a narrow (<1 mm) zone of very high activity within the cement matrix peaking on, or within, 1 mm of the well wall (feature ‘x’; Fig. 9b) beyond which activity levels fall rapidly over a distance of about 4 mm. Sur-prisingly, the zone of high 99Tc enrichment occurs only to one side of the
well (Fig. 9b(ii)), pointing towards disturbance of the sample during the experiment or a discontinuity, whether structural, mineralogical or chemical, in the sample. The autoradiography also shows that there is a significant amount of activity remaining within the well itself, which is also asymmetrically distributed to the same side of the well as the enrichment in the wall. This resembles some sort of gravitational sedi-ment (or precipitate) deposition feature on this side of the cesedi-ment block. The duplicate PFA:OPC sample was sectioned in order to investigate this
apparent artefact; identical results were obtained (Fig. S3 in Supple-mentary Information).
The results above demonstrate that the capacity to retard technetium migration varies substantially among different cement formulations. The five HCP appear to fall into two distinct groups. The first displays conventional diffusive transport behaviour whereby the relative affinity of 99Tc for the solid matrix increases from NRVB, through GGBS:OPC to
CEM I. This results in chromatographic breakthrough into the solution surrounding the cement blocks and regular symmetrical profiles in the autoradiographs. It can be explained by reversible exchange of 99TcO4
on C–S–H and AFm phases. Autoradiographs for the second group, comprising PFA:OPC and the Cebama reference blend, show high con-centrations of Tc in narrow zones with limited evidence of further migration into the matrix. No breakthrough at all occurred for the Cebama reference blend, suggesting the in situ formation of a Tc- containing precipitate, probably due to reduction of Tc(VII) to Tc(IV). Although early breakthrough was observed for PFA:OPC, it decreased markedly over the course of the experiment. This apparently anomalous type of behaviour could be explained by the existence of a physical defect allowing fast transit that was subsequently blocked or, more
plausibly, slower reaction kinetics for the precipitation process. Further work is required to characterise the zone of enhanced technetium uptake and identify the phase (or phases) responsible for immobilisation in these cement systems.
Batch experiments on individual mineral phases present in OPC and blended cements point to preferential but limited uptake of pertechne-tate by pure (Fe-free) C–S–H and AFm, and no significant adsorption onto ettringite or calcium aluminates. The exchange process is rapid, reaching equilibrium in a few hours. Based on the distribution ratios determined for these phases and hardened cement pastes, technetium (VII) is expected to be mobile in cementitious materials, provided no reducing agents are present to promote precipitation in the form of Tc (IV). The results are borne out by through-diffusion tests on intact, monolithic cement blocks where markedly different migration rates and behaviour were observed, primarily due to chemical interactions with the cement matrix rather than differential permeability or other physical factors. A backfill cement, developed specifically for the purpose of
Fig. 6. Elution curves for 99Tc in through-diffusion experiments on NRVB, CEM I and PFA:OPC. Insert shows changes over the first seven days.
radionuclide retention (NRVB), gave by far the poorest performance of all formulations studied in terms of both transport rates and overall technetium retention. Two of the matrices, PFA:OPC and a low-pH blend incorporating fly ash, effectively retarded Tc migration via precipitation in narrow, reactive zones. The findings have important implications
when choosing cementitious grouts and/or backfill for Tc-containing radioactive wastes.
Fig. 8. LPSL autoradiography results for (a) NRVB, (b) CEM I and (c) GGBS:OPC. Each diagram shows: (i) a photograph of the longitudinally sawn surface of the cement block; (ii) corresponding 16-colour contoured linearised LPSL autoradiograph; (iii) profile of the variation in radioactivity across the block, measured along the ‘lane’ drawn in (ii). For CEM I (b), the locations of rare, discrete ‘hots-spots’ of radioactivity (labelled ‘x’ and ‘y’) are shown in the corresponding LPSL auto-radiograph. (For interpretation of the references to colour in this figure legend, the reader is referred to the Web version of this article.)
Fig. 9. LPSL autoradiography results for (a) Cebama reference blend and (b) PFA:OPC cement blocks. Each diagram shows: (i) photograph of the longitudinally sawn surface of the cement block; (ii) corresponding 16-colour contoured linearised LPSL autoradiograph; (iii) profile of the variation in radioactivity across the block, measured along the ‘lane’ drawn in (ii). In PFA-OPC (ii), radioactivity is concentrated only on one side of the well (‘x’). In the Cebama reference blend block, the peak in radioactivity (y) is located within the cement and very close to the well wall. (For interpretation of the references to colour in this figure legend, the reader is referred to the Web version of this article.)
Declaration of competing interest
The authors declare that they have no known competing financial interests or personal relationships that could have appeared to influence the work reported in this paper.
The research described in this paper has received funding from the European Union’s Horizon 2020 Research and Training Programme of the European Atomic Energy Community (EURATOM) (H2020-NFRP- 2014/2015) under grant agreement no 662147 (CEBAMA). We would like to thank Dr Marcus Altmaier of Forschungszentrum Karlsruhe and his colleagues for their invaluable support. Tapio Vehmas and Markku Leivo from VTT Technical Research Centre of Finland are acknowledged for providing samples and constituents of the Cebama low-pH reference cement paste. We would also like to acknowledge the help of colleagues in the Nuclear Metrology Group at the National Physical Laboratory, in particular Elsje van Es, Peter Ivanov and Lynsey Keighley.
Appendix A. Supplementary data
Supplementary data to this article can be found online at https://doi. org/10.1016/j.apgeochem.2020.104580.
Allen, P.G., Shuh, D.K., Bucher, J.J., Edelstein, N.M., Reich, T., Denecke, M.A., Nitsche, H., 1997a. Chemical speciation studies of radionuclides by XAFS. J. Phys. IV
Allen, P.G., Siemering, G.S., Shuh, D.K., Bucher, J.J., Edelstein, N.M., Langton, C.A., Clark, S.B., Reich, T., Denecke, M.A., 1997b. Technetium speciation in cement waste forms determined by X-ray absorption fine structure spectroscopy. Radiochim. Acta
Amersham Biosciences, 2005. ImageQuant TL v.2005. Amersham Biosciences. GE
Angus, M., Borwick, J, Cann, G, 2011. The specification of cement powders for waste encapsulation processes at the Sellafield site. In: Proceedings of NUWCEM 2011,
Avignon, France. INIS IAEA, Vienna, Austria, pp. 48–58.
Atkins, M., Glasser, F.P., Kindness, A., 1992. Cement hydrate phases: solubility at 25�C.
Cement Concr. Res. 22, 241–246.
Atkins, M., Macphee, D., Kindness, A., Glasser, F.P., 1991. Solubility properties of ternary and quaternary compounds in the calcia-alumina-sulfur trioxide-water system.
Cement Concr. Res. 21, 991–998.
Baur, I., Keller, P., Mavrocordatos, D., Wehrli, B., Johnson, C.A., 2004. Dissolution- precipitation behaviour of ettringite, monosulfate and calcium silicate hydrate.
Cement Concr. Res. 34, 341–348.
Berner, U., 1999. Concentration limits in the cement based Swiss repository for long-
lived, intermediate-level radioactive wastes (LMA). PSI Bericht, 99-10.
Bel, J.J., Wickham, S.M., Gens, R.M., 2006. Development of the Supercontainer design for deep geological disposal of high-level heat emitting radioactive waste in Belgium.
Mater. Res. Soc. Symp. Proc. 932, 122.1.
Bonhoure, I., Scheidegger, A.M., Wieland, E., Dahn, R., 2002. Iodine species uptake by cement and C-S-H studied by I K-edge X-ray absorption spectroscopy. Radiochim.
Acta 90, 647–651.
Brodda, B.G., Xu, M., 1989. Leaching of chlorine, cesium, strontium and technetium from cement-fixed intermediate level liquid waste. Mater. Res. Soc. Symp. Proc. 127,
Brown, D.A., Chadwick, M.B., Capote, R., Kahler, A.C., Trkov, A., Herman, M.W., Sonzogni, A.A., Danon, Y., Carlson, A.D., Dunn, M., Smith, D.L., Hale, G.M., Arbanas, G., Arcilla, R., Bates, C.R., Beck, B., Becker, Brown, F., Casperson, R.J., Conlin, J., Cullen, D.E., Descalle, M.-A., Firestone, R., Gaines, T., Guber, K.H., Hawari, A.I., Holmes, J., Johnson, T.D., Kawano, T., Kiedrowski, B.C., Koning, A.J., Kopecky, S., Leal, L., Lestone, J.P., Lubitz, C., Marquez Damian, J.I., Mattoon, C.M., McCutchan, E.A., Mughabghab, S., Navratil, P., Neudecker, D., Nobre, G.P.A., Noguere, G., Paris, M., Pigni, M.T., Plompen, A.J., Pritychenko, B., Pronyaev, V.G., Roubtsov, D., Rochman, D., Romano, P., Schillebeeckx, P., Simakov, S., Sin, M., Sirakov, I., Sleaford, B., Sobes, V., Soukhovitskii, E.S., Stetcu, I., Talou, P., Thompson, I., van der Marck, S., Welser-Sherrill, L., Wiarda, D., White, M., Wormald, J.L., Wright, R.Q., Zerkle, M., Zerovnik, G., Zhu, Y., 2018. ENDF/B-VIII.0:
the 8th major release of the Nuclear Reaction Data Library with CIELO-project cross
sections, new standards and thermal scattering data. Nucl. Data Sheets 148, 1-142.
Bruno, J., Ewing, R.C., 2006. Spent nuclear fuel. Elements 2, 343–349.
Burke, I.T., Boothman, C., Lloyd, J.R., Mortimer, R.J.G., Livens, F.R., Morris, K., 2005. Effects of progressive anoxia on the solubility of technetium in sediments. Environ.
Sci. Technol. 39, 4109–4116.
Carbol, P., Wegen, D.H., Wiss, T., Fors, P., 2012. Spent fuel as waste material. Compr.
Nucl. Mater. 5, 389–420.
Childs, B.C., Poineau, F., Czerwinski, K.R., Sattelberger, A.P., 2015. The nature of the volatile technetium species formed during vitrification of borosilicate glass.
J. Radioanal. Nucl. Chem. 306, 417–421.
Cathelin, R., 2012. Linearize GelData. Sigenae team, INTRA. Toulouse, France. http://
Corkhill, C.L., Bridge, J.W., Hillel, P., Gardner, L.J., Banwart, S.A., Hyatt, N.C., 2012. Technetium-99m transport and immobilisation in porous media: development of a
novel nuclear imaging technique. Mater. Res. Soc. Symp. Proc. 1518, 123–129.
Cui, D., Eriksen, T.E., 1996. Reduction of pertechnetate in solution by heterogeneous electron transfer from Fe(II)-containing geological material. Environ. Sci. Technol.
Eriksen, T.E., Ndalamba, P., Cui, D., Bruno, J., Caceci, M., Spahiu, K., 1993. Solubility of
the Redox-Sensitive Radionuclides 99Tc and 237Np under Reducing Conditions in
Neutral to Alkaline Solutions. Effect of Carbonate. Svensk K€arnbr€anslehantering AB,
Stockholm, Sweden, p. 32. SKB Technical Report, TR-93-18.
Evans, N.D.M., 2008. Binding mechanisms of radionuclides to cement. Cement Concr.
Res. 38, 543–553.
Felipe-Sotelo, M., Hinchliff, J., Drury, D., Evans, N.D.M., Williams, S., Read, D., 2014. Radial diffusion of radiocaesium and radioiodide through cementitious backfill.
Phys. Chem. Earth 70–71, 60–70.
Felipe-Sotelo, M., Hinchliff, J., Evans, N.D.M., Read, D., 2016a. Solubility constraints affecting the migration of selenium through the cementitious backfill of a geological
disposal facility. J. Hazard Mater. 305, 21–29.
Felipe-Sotelo, M., Hinchliff, J., Field, L.P., Milodowski, A.E., Holt, J.D., Taylor, S.E., Read, D., 2016b. The solubility of nickel and its migration through the cementitious backfill of a geological disposal facility for nuclear waste. J. Hazard Mater. 314,
Giffaut, E., Griv�e, M., Blanc, Ph, Vieillard, Ph, Col�as, E., Gailhanou, H., Gaboreau, S., Marty, N., Mad�e, B., Duro, L., 2014. ANDRA thermodynamic database for
performance assessment: ThermoChimie. Appl. Geochem. 49, 225–236.
Gilliam, T.M., Spence, R.D., Bostick, W.D., Shoemaker, J.L., 1990. Proceedings of the gulf coast hazardous substance research center second annual symposium: mechanisms and applications of solidification/stabilization of technetium in cement-based
grouts. J. Hazard Mater. 24, 189–197.
Glasser, F.P., 2011. Application of inorganic cements to the conditioning and immobilisation of radioactive wastes. In: Ojovan, M.I. (Ed.), Handbook of Advanced
Radioactive Waste Conditioning Technologies. Woodhead, pp. 67–135.
Gonzalez, A.L., Li, H., Mitch, M., Tolk, N., Duggan, D.M., 2002. Energy response of an
imaging plate exposed to standard beta sources. Appl. Radiat. Isot. 57, 875–882.
Grambow, B., L�opez-García, M., Olmeda, J., Griv�e, M., Marty, N.C.M., Grangeon, S., Claret, F., Lange, S., Deissmann, G., Klinkenberg, M., Bosbach, D., Bucur, C., Florea, I., Dobrin, R., Isaacs, M., Read, D., Kittnerov�a, J., Drtinov�a, B., Vop�alka, D., Cevirim-Papaioannou, N., Ait-Mouheb, N., Gaona, X., Altmaier, M., Nedyalkova, L., Lothenbach, B., Tits, J., Landesman, C., Rasamimanana, S., Ribet, S., 2020. Retention of radionuclides on cementitious systems: main outcome of the CEBAMA project.
Appl. Geochem. (this issue).
Griv�e, M., Duro, L., Col�as, E., Giffaut, E., 2015. Thermodynamic data selection applied to radionuclides and chemotoxic elements: an overview of the ThermoChimie-TDB.
Appl. Geochem. 55, 85–94.
Hallam, R.J., Jain, S.L., Evans, N., 2011. Sorption of Tc(IV) to cementitious materials associated with a geological disposal facility for radioactive waste. In: Proc. Waste
Management 2011 Conf (Phoenix, Arizona, USA).
Hawthorne, F.C., Krivovichev, S.V., Burns, P.C., 2000. The crystal chemistry of sulfate
minerals. Rev. Mineral. 40, 1-112.
Hoch, A.R., Baston, G.M.N., Glasser, F.P., Hunter, F.M.I., Smith, V., 2012. Modelling evolution in the near field of a cementitious repository. Mineral. Mag. 76,
Idiart, A. (Ed.), 2017. Preliminary Results and Interpretation of the Modelling of WP1 & WP2 Experiments, CEBAMA Deliverable D3.05, p. 70. http://www.cebama.eu/home
Isaacs, M., Hayes, M., Rawlinson, S., Angus, M., Qaisar, A., Christie, S., Edmondson, S., Read, D., 2018. The processing and product characteristics of a blended cement grout incorporating a polycarboxylate ether superplasticiser. Adv. Cement Res. 30,
Jantzen, C., Johnson, A., Read, D., Stegemann, J., 2010. Cements in waste management.
Adv. Cement Res. 22, 225–231.
Kim, D., Kruger, A.A., 2018. Volatile species of technetium and rhenium during waste
vitrification. J. Non-Cryst. Solids 481, 41–50.
Kleykamp, H., 1988. The chemical state of fission products in oxide fuels at different
stages of the nuclear fuel cycle. Nucl. Technol. 80, 412–422.
Lange, S., 2019. Structural Uptake and Retention of Safety Relevant Radionuclides by
Cementitious Materials. PhD thesis. RWTH Aachen University.
Lange, S., Kowalski, P., P�seni�cka, M., Klinkenberg, M., Rohmen, S., Bosbach, D.,
Deissmann, G., 2018. Uptake of 226Ra in cementitious systems: a complementary
solution chemistry and atomistic simulation study. Appl. Geochem. 96, 204–216.
Leblans, P., Vandenbroucke, D., Willems, P., 2011. Storage phosphors for medical
imaging. Materials 4, 1034–1086.
Lewis, B.J., Thompson, W.T., Iglesias, F.C., 2012. Fission product chemistry in oxide
fuels. Compr. Nucl. Mater. 2, 515–546.
Lloyd, J., Sole, V., van Praagh, C., Lovley, D., 2000. Direct and Fe(II)-mediated reduction
of technetium by Fe(II)-reducing bacteria. Environ. Microbiol. 66, 3743–3749.
Lukens, W.W., Shuh, D.K., Muller, I.S., McKeown, D.A., 2003. X-ray absorption fine structure studies of speciation of technetium in borosilicate glasses. Mater. Res. Soc.
Symp. Proc. 802. DD3.3.1-DD3.3.6.
Luksic, S.A., Riley, B.J., Schweiger, M., Hrma, P., 2015. Incorporating technetium in
Ma, B., Fernandez-Martinez, A., Findling, N., Koishi, A., Tisserand, D., Bureau, S., Charlet, L., Grangeon, S., Tournassat, C., Claret, F., Marty, N.C.M., Salas-Colera, E., Elkaim, E., Marini, C., 2017. Evidence of multiple sorption modes in layered double
hydroxides using Mo as structural probe. Environ. Sci. Technol. 51, 5531–5540.
Ma, B., Charlet, L., Fernandez-Martinez, A., Kang, M., Mad�e, B., 2019. A review of the retention mechanisms of redox-sensitive radionuclides in multi-barrier systems.
Appl. Geochem. 100, 414–431.
Masters-Waage, N.K., Morris, K., Lloyd, J.R., Shaw, S., Mosselmans, J.F.W.,
Boothman, C., Bots, P., Rizoulis, A., Livens, F.R., Gareth, T.W., Law, G.T.W., 2017. Impacts of repeated redox cycling on technetium mobility in the environment.
Environ. Sci. Technol. 51, 14301–14310.
Matschei, T., Lothenbach, B., Glasser, F.P., 2006. The AFm phase in Portland cement.
Cement Concr. Res. 37, 118–130.
Mattigod, S.V., Whyatt, G.A., Serne, R.J., Martin, P.F., Schwab, K.E., Wood, M.I., 2001. Diffusion and Leaching of Selected Radionuclides (Iodine-129, Technetium-99, and Uranium) through Category 3 Waste Encasement Concrete and Soil Fill Material. Pacific Northwest National Laboratory (PNNL), PNNL-13639. Richland, WA (United
Mattigod, S.V., Whyatt, G.A., Serne, J.R., Wood, M.I., 2004. Diffusion of iodine and technetium-99 through waste encasement concrete and unsaturated soil fill material.
Mater. Res. Soc. Symp. Proc. 824, 391–398.
Milodowski, A.E., Rochelle, C.A., Purser, G., 2013. Uptake and retardation of Cl during
cement carbonation. Procedia Earth Planetary Sci 7, 594–597.
NAGRA, 2002. Project Opalinus Clay - Safety Report. Demonstration of Disposal Feasibility for Spent Fuel, Vitrified High-Level Waste and Long-Lived Intermediate-
Level Waste (Entsorgungsnachweis). NAGRA Technical Report 02-05, Wettingen.
NAGRA, 2008. Entsorgungsprogramm 2008 der Entsorgungspflichtigen. NAGRA
Technischer Bericht 08-01. Wettingen.
Ochs, M., Mallants, D., Wang, L., 2016. Radionuclide and Metal Sorption on Cement and
Concrete. Springer, p. 301.
Pegg, I.L., 2015. Behavior of technetium in nuclear waste vitrification processes.
J. Radioanal. Nucl. Chem. 305, 287–292.
Posiva, 2012. Safety Case for the Disposal of Spent Nuclear Fuel at Olkiluoto. Posiva
Rasband, W.S., 2013. ImageJ v.1.48k (15 December 2013. US National Institutes of Health, Bethesda, Maryland, USA, 1997-2016. http://rsb.info.nih.gov/ij.
Saslow, S.A., Um, W., Russell, R.L., Williams, B.D., Assmussen, R.M., Varga, T., Qafoku, O., Riley, B.J., Lawter, A.R., Snyder, M.M.V., Baum, S.R., Leavy, I.I., 2018. Effluent Management Facility Evaporator Bottoms: Waste Streams Formulation and Waste Form Qualification Testing. Pacific Northwest National Lab. (PNNL), PNNL-
26570. Richland, WA (United States).
Schulte, E., Scoppa, P., 1987. Sources and behaviour of technetium in the environment.
Sci. Total Environ. 64, 163–179.
SKB, 2015. Safety Analysis for SFR Long-Term Safety: Main Report for the Safety
Assessment SR-PSU. Svensk K€arnbr€anslehantering AB.
Shannon, R.D., 1976. Revised effective ionic radii and systematic studies of interatomic
distances in halides and chalcogenides. Acta Crystallogr. A 32, 751–767.
Smith, R.W., Walton, J.C., 1993. The role of oxygen diffusion in the release of technetium
from reducing cementitious waste forms. Mater. Res. Soc. Symp. Proc. 294, 247–253.
Tallent, O.K., McDaniel, E.W., Cul, G.D.D., Dodson, K.E., Trotter, D.R., 1987. Immobilization of technetium and nitrate in cement-based materials. Mater. Res.
Soc. Symp. Proc. 112, 23–32.
Takahashi, K., 2002. Progress in science and technology on photostimulable BaFX:Eu2þ
(X¼Cl, Br, I) and imaging plates. J. Lumin. 100, 307–315.
van Es, E., Hinchliff, J., Felipe-Sotelo, M., Milodowski, A.E., Field, L.P., Evans, N.D.M., Read, D., 2015. Retention of chlorine-36 by a cementitious backfill. Mineral. Mag.
Vehmas, T., Montoya, V., Cruz Alonso, M., Va�sí�cek, R., Rastrick, E., Gaboreau, S., Ve�cerník, P., Leivo, M., Holt, E., Ait Mouheb, N., Finck, N., Schild, D., Sch€afer, T., Adam, C., Dardenne, K., Rothe, J., Fernandez, A., Garcia-Calvo, J.L., Felipe- Sotelo, M., Svoboda, J., Isaacs, M., Read, D., �Cervinka, R., Rosendorf, T., Vasconcelos, R., Provis, J., Hyatt, N., Corkhill, C., 2020. Slag containing low-pH cementitious materials for deep underground nuclear waste repositories. Appl.
Vehmas, T., Schnidler, A., L€oija, M., Leivo, M., Holt, E., 2017. Reference mix design and castings for low-pH concrete for nuclear waste repositories. KIT Sci. Rep. 7734,
Verhoef, E.V., de Bruin, A.M.G., Wiegers, R.B., Neeft, E.A.C., Deissmann, G., 2014. Cementitious Materials in OPERA Disposal Concept in Boom Clay. Report OPERA-
PG-Cov020. COVRA, Vlissingen.
Warwick, P., Aldridge, P., Evans, N., Vines, S., 2007. The solubility of technetium (IV) at
high pH. Radiochim. Acta 95, 709–716.
Weaver, J., Soderquist, C.Z., Washton, N.M., Lipton, A.S., Gassman, P.L., Lukens, W.W., Kruger, A.A., Wall, N.A., McCloy, J.S., 2017. Chemical trends in solid alkali
pertechnetates. Inorg. Chem. 56, 2533–2544.
Westsik Jr., J, Cantrell, K, Serne, R, Qafoku, N, 2014. Technetium Immobilization Forms:
Literature Survey, , EMSP-RPT-023PNNL-23329. US DoE.
Wieland, E, Tits, J, Spieler, P, Dobler, J, 1998. Interaction of Eu(III) and Th(IV) with
sulfate-resisting portland cement. Mater. Res. Soc. Symp. Proc. 506, 573–578.
Wildung, R., McFadden, K., Garland, T., 1978. Technetium sources and behaviour in the
environment. J. Environ. Qual. 8, 156–161.
Zeissler, C.J., 1997. Comparison of semiconductor pixel array, phosphor plate, and track- etch detectors for alpha autoradiography. Nucl. Instrum. Methods Phys. Res. A392,